Fig. 7: Solar cell parameters of TCO/a-Si:H(n)/c- Si(p) solar cells with variing gas phase doping concentrations of the a-Si:H layer. 2000 ppm. The open circuit voltage follows the same trend as the efficiency. Also the short circuit current increases with increasing NG until NG = 2000 ppm and stays approximately constant with a further increase of NG. This result can be interpreted as follows. It is well known that substitutional doping of a-Si:H on glass substrates leads to the creation of deep defects. This leads to a self compensation effect in a-Si:H. However, the maximum conductivity for P-doped a-Si:H is reported for NG = 10 000 ppm  a result that is supported by our findings (Fig. 6). For amorphous silicon on crystalline silicon the initial growth of a-Si:H might be different to the case of a-Si:H on glass substrates. Due to the doping defects are created which are located at the interface and in the a-Si:H layer. The optimal gas phase doping concentration is obtained when the Fermi energy in the a-Si:H layer is sufficiently close to the conduction band and the defect density is still considerably low. Obviously the optimum gas phase doping concentration for a-Si:H/c-Si solar cells is about 2000 ppm. Using optimized deposition conditions a maximum efficiency of 17% on a flat c-Si substrate with diffused back surface field was obtained (Fig. 8). For this J (mA/cm 2 ) J SC (mA/cm 2 ) V oc (V) η(%) 0 20 40 32 30 28 0.6 0.5 0.4 12 10 8 (c) (b) (a) 0 2000 4000 6000 8000 10000 [SiH ]/[PH ](ppm) 4 3 a-Si:H(n, i)/c-Si(p)/c-Si (p + ) η= 17% a-Si:H(n)/c-Si(p)/a-Si:H (p + ) η= 17.2% Fig. 8: Best solar cells using a diffused BSF (c-Si(p + 0.0 -0.2 -0.4 U (V) -0.6 -0.8 )) and a low temperature a-Si:H(p) BSF. 1228 heterojunction solar cell a thin (3nm) intrinsic amorphous layer was used. Additionally we fabricated solar cells with a-Si:H(p) back surface field on a textured substrate but without special antireflex coating using only low temperature process steps. Without an intrisic a-Si:H layer a maximum efficiency of 17.2 % was obtained (see Fig. 8). This is the highest efficiency of a complete low temperature a-Si:H(n)/c-Si(p)/a-Si:H(p) solar cell reported so far. CONCLUSION The basic electronic properties of a a-Si:H/c-Si heterojunction were meaured using PEYS and SPV. The valence band offset was determined to 0.45 eV. Simulations show that the interface states density of a a- Si:H(n)/c-Si(p) has a major impact on the cell efficiency and must be as low as possible. For the inverse doping structure Dit plays a minor role. However, with a Dit of about 2×10 11 cm -2 eV -1 a high efficiency TCO/Si:H(n)/c-Si(p) cell is achievable. Using optimized deposition conditions with respect ot the depostion temperature and the gas phase doping concentration a complete low temperature processed solar cell with an efficiency above 17 % was processed. ACKNOWLEDGEMENTS This work is supported by the Bundisministerium für Bildung und Forschung. Contract number FKZ01F0012-19 REFERENCES  M. Tanaka, M. Taguchi, T. Matsuyama, T. Sawada, S. Tsuda, S. Nakano, H. Hanafusa, Y. Kuwano, “Development of New a-Si/c-Si Heterojunction Solar Cells”, Jpn. J. Appl. Phys 31, 1993, p. 3518.  M. Schmidt, A. Schoepke, L. Korte, O. Milch, W. Fuhs, “The gap state density distribution in extremely thin a-Si:H layers on crystalline silicon wafers “, J. Non-Cryst. Solids 338-340, 2004, p. 211.  Y. W. Lam, “Surface-state density and surface potential in MIS capacitors by surface photovoltage measurements”, J. Phys. D: Appl. Phy.s 4, 1971, p1370.  K. Winer and L. Ley, “Surface states and exponential valence band tail in a-Si:H”, Phys. Rev. B 36, 1987, p. 6072.  R. Stangl, A. Froitzheim, L. Elstner, M., Schmidt, . Fuhs, “Amorphous/Crystalline Silicon Heterojunction Solar Cells, a Simulation Study“, Proc. 17 th EPVSEC, Munich, 2001, p. 1387.  W. E. Spear and P. G. LeComber , “Substitutional doping of amorphous silicon”, Solid State Commun. 17, 1975, p.1193.